ACTA PHYSICA POLONICA A Vol. 124 (2013) No. 2 Special Anniversary Issue: Professor Jan Czochralski Year 2013 Invited Paper Czochralski-Grown Silicon Crystals for Microelectronics A. Bukowski Institute of Electronic Materials Technology, Wólczy«ska 133, 01-919 Warsaw, Poland The Czochralski method of crystal growth is used since 1950s in scientic and industrial laboratories for growth of single crystals of large size and high quality. The article presents the general characteristics and selected improvements of the Czochralski method, and discusses its meaning and advantages in growth of silicon single crystals playing a key role in microelectronics. DOI: 10.12693/APhysPolA.124.235 PACS: 81.10.Fq, 85.40.e resources (the primary resource of silicon is SiO2 ). 1. The Czochralski method of silicon Silicon has a unique characteristics of forming, on crystallization its surface, an ultrathin passivating oxide lm. Ther- In the era of semiconductor electronics, monocrys- mal conductivity of silicon (140163 W/(m K)) is higher talline silicon remains a basic and widely used material in comparison to other semiconductors (GaAs 46 . It will probably continue to dominate in the world 55 W/(m K), SiC 1655 W/(m K)). This property is of of electronics for many years to come. The rst material particular signicance as it leads to (advantageous) heat in history, though, on the basis of which the invention of dissipation at semiconductor junctions. a transistor was made (1948) was germanium (Ge). In a leading material in electronics due to its energy gap order to produce a germanium single crystal, the molten (1.1 eV at 300 K) which guarantees the work of semicon- germanium was held in a graphite crucible, and the crys- ductor devices at high temperatures. Silicon became tal grew from a seed initially immersed in the liquid and later slowly pulled upwards. This method of crystalliza- 2. Growth process of silicon single crystals: tion was described in 1916 by Jan Czochralski, a scien- basic parameters tist and inventor (for his life and scientic achievements, see ). During the rst years after invention, Czochralski focused his studies on determination of the rate of metal crystallization. In later investigations, he proved that materials produced using this method are single crystals. They were not single crystals in today understanding, though, they were threads of such metals as zinc, tin and lead. At the time there was no need whatsoever for monocrystaline materials, as all materials indus- From the point of view of crystallization, the Czochralski method is classied as a directional crystallization process. tures; recrystallization, mostly in order to improve the mechanical properties. Returning to the subject of this article, it must be pointed out that despite technological progress and development in the examination of semiconductor devices, the Czochralski crystallization method applied to semiconductor materials, in particular to silicon, remained essentially the same since the 1950s. It is commonly called If the crystal is doped, then the dopant concentration varies along its axis. The distribution of the dopant together with in- creasing solid:liquid proportion is described by the following formula : C = kC0 (1 − g)k−1 , trially exploited at that time were polycrystalline. Properties were studied such as textures, martensitic struc- During growth, the total mass of the mate- rial (liquid plus crystal) is conserved. where C dopant concentration, dopant distribution, C0 k coecient of concentration of the dopant before the beginning of the process, g the crystallized material to charge ratio. General characteristics of commercially grown silicon single crystals includes the data on typical dopants, crystal orientation, growth rate and other technological parameters as well as on the quality and purity: the Czochralski method (for a detailed description of the method see, e.g. ). On the following pages, the char- Technological parameters: • acteristics of the method, contributing to its success are discussed, taking into consideration the mechanisms of crystallization and technological progress observed in the mony (Sb) and arsenic (As), • tronics and microelectronics. At the present time, silicon • Atmosphere: most often argon (Ar). Gas ow rate 10200 Tr. ally. The broad use of silicon is due to both, its physical (235) h111i, h100i, h110i, of 1550 l/min most often in exhaust vacuum of crystals are produced in tens of thousands of tons, annuand technological characteristics as well as availability of Crystal growth directions: h112i, last decades. The discussion is focused on crystallization of silicon, a material which became irreplaceable in elec- Typical dopants: boron (B), phosphorus (P), anti- • Rate of crystallization: 0.52.0 mm/min, A. Bukowski 236 • • The charge and crystal diameter: up to 150 kg and such as: high vacuum technology, methods of pure argon 300 mm, respectively, production, methods of tightness assessment of installa- Homogeneous temperature distribution: through both, the crucible rotation achieved (usually 320 rpm) and rotation of pulling rod (with a Si seed attached) rotation (usually 530 rpm), • Crucible material: • usually pure melted quartz the pulling rod, computerization of processes etc. Taking into consideration the above requirements the what are the advantages of the Czochralski method? There are only three methods of crystallization: the Czochralski method (Cz), the oating zone (FZ) method Material of heater and container for quartz crucible: and the Verneuil method (MV), which fulll the con- high purity graphite, dition that the growing crystal has no contact with the Liquid level during growth: typically, automated maintenance of a xed level of the liquid is applied. Typical structural quality: dislocation-free crystal. • Usual carbon content: growth of silicon single crystals and ensure full repeata- crystallization and varies from a few to over ten centimeters. Such a large distance ensures a strong reduction of nucleation centers formation. 3 at./cm , Another particular feature of the Czochralski method is the control of the diameter of the single crystal not only Usual oxygen content: 5×1017 < O2 < 9×1017 lization, two (Czochralski and oating zone) are useful for wall of the crucible is usually outlying from the area of • < 2×1016 crucible material. Among these three methods of crystal- bility of the growth process. The area of contact with the Characteristics of grown Si crystals: • stability processes, stability of movement parameters of fulllment of which is not easy, the question remains: (rarely synthetic quartz), • tions and furnaces, electronic solutions of temperature by changing the power of the heater, but also by chang- 3 at./cm . ing the pulling rate or by changing the rotation speed of crucible or of the crystal. 3. Silicon crystal growth process requirements. Characteristics of the Czochralski method ◦ Silicon (melting point 1415 C) reacts with oxygen and water vapor if they are present, even in trace amounts, in the furnace atmosphere. It also enters into a live reaction with crucible materials. In order to avoid oxidation of the charge, it is necessary to use a protective atmosphere, i.e. In the case of changing the pulling rate, the crystallization heat is emitted or absorbed, inuencing the diameter of the growing crystal. This phenomenon does not occur when material crystallizes using a dierent method based on direct crystallization in a crucible. Appropriate manipulation or application of programming of the above-listed parameters not only changes the diameter of the growing crystal, but also activate or limit the nucleation centers. argon or he- lium with minimized oxygen and water vapor content. 4. Improvements of the Czochralski method Molten silicon is an aggressive material, which dissolves applied to silicon the quartz crucible. The quartz crucible is a source of oxygen created due to the reaction of molten silicon with Modern microelectronics requires silicon single crystals The dissolved oxygen partially leaves the liq- of a standard 200 mm diameter (the state of the art tech- uid and moves to the furnace atmosphere, and forms the nologies are starting to use the crystals of 300 mm diam- silicon monoxide. eter). The mass of 1 m long crystals exceeds 50 kg. The quartz. During the growth process, precipi- tate nucleation centers from foreign phases (i.e. silicon quartz crucibles used in the growth process have a diam- 00 (≈ 450−600 monoxide) aect the growth process. When such centers eter of 1824 exist, the crystal continues to grow as a polycrystal. To charge, disadvantageous phenomena tend to occur, such ascertain a successful growth process, the formation of as: the nucleation centers must be minimized. A particular solution which reduces the nucleation centers formation • stream, it is injected as if the smoke into a chimney and it • Overheating of quartz crucibles is observed for crucibles of increased diameter and when the distance is removed from the bottom part of the furnace using the from the wall of the crucible to the side of growing suitable vacuum pumps. This is a particular solution the single crystals is large; aim of which is to remove the nucleation centers (due to the presence of silicon vapor, silicon monoxide, and vapor Thermal turbulences appear in molten silicon of a large mass; is the direction of argon ow through the furnace. The gas is forced through the furnace against the convection mm). With increasing silicon • of dopants such as phosphorus, antimony and other con- The large amount of molten silicon in itself has a negative inuence on the crystal puller; taminations occurring at the crystallization front) from the area of crystallization. Facing the above dened difculties requires application of various high-technologies • Large electric power is needed to maintain a large mass of silicon in molten state. Czochralski-Grown Silicon Crystals for Microelectronics 237 These factors entail large costs and cause diculties in Due to the use of two congurations simultaneously, maintaining the high quality of single crystals. There are the magnetic elds described in (c) and (e), are called a few directions of improvement of the growth process of second-generation magnetic elds. large crystals. Up to now, the studies of magnetic eld application The rst one is a group of improvements without have been mostly focused on the congurations (a), (b) changing the construction of the puller, for example using and (c). more than one heater, ameliorating the quartz crucibles, follows. using new types of thermal insulation, constructional improvements of heating elements, etc. Other improvements are more complex. Two of them are described below: • Magnetic-eld-applied Czochralski (MCZ), leading and consequently causing an improvement of single-crystal quality. When applying a relatively strong magnetic eld such as 0.60.8 T, a signicant decrease of oxygen content in If such strong magnetic eld is used, the processes are dicult to carry out because of problems related to the ow of heat from the heater to the crystallization area. The costs related to the application of such magnetic eld are high. When a weaker magnetic eld is applied (up to 0.05 T) thermal convec- Continuous liquid feed method (CLF method), resulting in an improvement of axial homogeneity of the single crystal. 4.1.1. Steady magnetic elds horizontal (a) the crystal is attained. to signicant reduction of the scale of turbulences, • Their characteristics can be summarized as The method enables to reduce the mass of molten silicon. tion was absent due to the rotation of the crucible and the seed crystal which is a signicant advantage of this conguration . 4.1.2. Axial magnetic eld (b) The temperature layers under the crystallization front 4.1. The Czochralski method with the application of a magnetic eld The use of a magnetic eld in silicon single crystal growth has a long history . Research in this area and the rst results of experiments were attained for single crystals of 76100 mm diameter. The main aim, a reduction of the amount of oxygen in the silicon single crystals, has been achieved. For a long time, a steady magnetic eld set horizontally (perpendicularly to the crucible axis) to the charge was used. In order to achieve the intended results, the intensity of the magnetic eld was relatively large and amounted to 0.6−0.8 T which required an additional electric power comparable to the heating power of the furnace, despite using moderate-size chambers of Czochralski furnace. The method was further developed using dierent congurations of magnetic eld, i.e.: this, the growth processes are easier to carry out. The homogeneity and oxygen reduction eects are dicult to achieve. Slowing down the oxygen diusion to the surface leads to an increased oxygen content in the grown crystals. Application of this conguration does not bring any advantages. 4.1.3. Unipolar magnetic eld (c) The lines of the magnetic eld are orthogonal in rela- tion to the bottom of the crucible and to its side. Due to this, the largest magnetohydrodynamic pressure occurs at the crucible walls, whereas small magnetic forces act on the area around the crystallization front. drop of oxygen value to the level of 2×1017 The 3 at./cm was achieved with magnetic eld of 0.1 T, which is the best result so far. Besides the above mentioned eects, application of the magnetic eld leads to a visible calming of the liquid surface. When the charge is large, vibrations of the ex- (a) Horizontal magnetic eld (mentioned above); (b) Axial magnetic eld (magnetic ux is parallel to the axis of the furnace and of the growing crystal); (c) Unipolar magnetic eld (the lines of the magnetic eld are perpendicular to the walls and to the bottom of the quartz crucible). are more symmetrical than in conguration (a). Due to This eect was at- tained thanks to the interaction of two independent axial elds; tended liquid surface occur as a harmful phenomenon. Elimination of the vibrations is an additional advantage of magnetic eld application. 4.2. Continuous liquid feed method Research regarding this method originates from the needs to achieve savings in the use of the quartz crucible [12, 14]. original charge. (d) Magneto-hydro-dynamic-rotor (MHD); Continuous feeding of the crucible with silicon leads to crystals of a mass larger than the mass of Theoretically, when using the continu- ous feeding, the crystal length is limited only by the time during which the quartz crucible remains intact. In prac- (e) Steady (axial) magnetic eld with a simultaneous interaction of MHD conguration. The aim is to tice, several silicon single crystals of total 100−200 kg mass are grown in a series of processes proceeded with- break down the cells of ow circulation which are out cooling the furnace. formed in the axial eld using the MHD congura- with polycrystalline rods, granules or silicon powder as The furnace may be charged tion. well as with molten silicon. A. Bukowski 238 A practical problem that arose, regarded the process pected to take place soon, as multiple possible magnetic- of a continuous feeding of melted silicon which caused -eld settings (especially the second generation elds) perturbations in the process of crystal growth. So far, give a big choice of congurations. Moreover, for mag- this method is used to produce silicon for solar applica- netic eld generations, superconducting magnets at liq- tions, where the requirements concerning crystal quality uid helium temperature can be used with a reduced power are not high. If the perturbation problem was solved, this cost. Good quality of silicon crystals produced using the method would become of interest for the single-crystal MCZ method prove that its application is eective. growth task. Furthermore, besides savings in the use the CLF method the main eorts regarding its imple- of the quartz crucible, this method opens the door to mentations and improvements are focused on the use of achieve a high homogeneity in axial distribution of the new materials, including, in particular, new crucible ma- dopant. The silicon feed which does not contain a dopant, terials. In will dissolve the concentrated dopant in the liquid found in the crucible. In the case of dopants with a decom- position coecient k < 1, a constant concentration of, e.g., phosphorus in silicon crystal may be expected. This phenomenon had been conrmed by experimental data. Crystallization at the conditions of strongly reduced volume of molten silicon in the crucible may become an even more valuable modication of the method. Here, the crucible will be fed with a silicon feed. In this case, the volume of the molten material will be a classical zone and the crystallization will be subject to zone crystallization instead of conventional Czochralski directional crystallization. Consequently, the dopant distribution will be determined by a dierent law. Up to now, such a version of the CLF method has not been reported, but the prerequisites of such a method seem to be justied. The advantage of this version would be to achieve ve times smaller volume of liquid in the crystallization area than while using the conventional method. Such or other improvements are expected to be developed in future. They can be concentrated around new crucible materials (i.e. silicon nitride, carbon based materials, other materials and their combinations, including modied quartz). Using such new materials may be fruitful for the success of the CLF method. 5. Summary In the article, the currently applied Czochralski technique of silicon single crystal production is presented. Multiple advantages of the method led to production of such crystals at an industrial scale. The increase of diameter of produced single crystals from 76100 mm to 200300 mm has been accompanied by various improvements, such as magnetic eld application and continuous liquid feeding. It is expected that such improvements will be introduced into commercial production practice. In particular, the introduction of magnetic elds is ex- References  Handbook of Semiconductor Silicon Technology, Eds. W.C.O. Mara, R.B. Herring, L.P. Hunt, Noyes Publications, Park Ridge (NJ) 1990.  H.R. Hu, J. Electrochem. Soc. 149, S35 (2002).  L. Arnberg, M. Di Sabatino, E. Øvrelid, JOM, 38 (October 2011).  G. Fisher, M.R. Seacrist, R.W. Standley, Proc. IEEE 100, 1454 (2012).  P. Tomaszewski, On Jan Czochralski, Atut, Wrocªaw 2012 (in Polish, the English translation in preparation).  Elementary Crystal Growth, Ed. K. Sangwal, Saan Publ., Lublin 1994.  D.T.J. Hurle, B. Cockayne, in: Handbook of Crystal Growth, Vol. 2A, Basic Techniques, Prentice-Hall, Englewood Clis 1994, Ch. 3.  A.A. Wheeler, in: Handbook of Crystal Growth, Vol 1b. ed. D.T.J. Hurle, North-Holland, Amsterdam 1993, p. 683.  W.G. Pfann, Zone Melting, Wiley, New York 1958.  M. Ohwa, T. Higuchi, E. Toji, M. Watanabe, K. Homma, S. Takasu, in: Semiconductor Silicon, Eds. H.R. Hu, T. Abe, B. Kolbesen, The Electrochemical Society, Pennington, NJ 1986, p. 117.  L.N. Hjellming, J.S. Walker, J. Fluid Mech. 182, 335 (1987).  A. Bukowski, P. Zabierowski, Elektronika 40, 10 (1999) (in Polish).  A. Bukowski, P. Zabierowski, W. Grzejszczyk, R. Nowak, Method of Obtaining the Silicon Single Crystals in the Czochralski Crystalization Device, Patent A1(21) 288359 (22) 90 12 20 5(51) C33B 15/00, 13.01.1994 (Polish patent).  Leybold System Presentation Silicon'96, Fifth Sci- entic and Bussiness Conf., Roºnov pod Radho²t¥m (Czech Republic) 1996.